Macromolecules 1994, 27, 3046-3052
Dewetting as a Probe of Polymer Mobility in Thin Films Gunter Reitert Max-Planck Institut f u r Polymerforschung, P.O. Box 3148, 6500 Mainz, Germany Received August 16, 1993; Revised Manuscript Received December 21, 1 9 9 6
ABSTRACT: Spin-coated polystyrene films thinner than the unperturbed size of the molecules on glass substrates were studied by X-ray reflectometry. Detailed knowledge about the dewetting process of these unstable films allowed to probe polymer dynamics in this confined geometry. The film thickness increased upon annealing reaching a stable value before dewetting st.arted. The thickness change translates into a decrease in polymer density. This decrease is larger the thinner the films are. Consequently, the polymer density depends on film thickness and reaches its bulk value only for films thicker than about the size of the unperturbed molecule. A quite distinct dependence of the onset of dewetting on film thickness was observed. For the thinnest films dewetting was completed at temperatures well below the glass transition temperature. As a consequence of the lower polymer density, the mobility of the molecules was increased. A tentative explanation of these effects based on packing considerations leading to inaccessible sites is given.
1. Introduction and commensurability with the wall but also packing considerations. Miniature devices and various applications like coatings, At present all theoretical treatments'~~ and computer lubrication, or electronic packaging demand progressively simulationsSl0 of confined polymer systems (melts) assume thinner polymeric films. In some cases the thickness of that the average density of a thin layer of macromolecules such films can be smaller than the unperturbed size of the is not deviating from its value in the bulk. This is probably macromolecules (in the following such films are called true if one looks at molecules close to an interface within thin). Confinement influences conformation and intera thick sample. However, if the molecules are confined twining of the molecules.' Structural changes induced by by two interfaces like in a thin film there is experimental the interaction with a solid substrate can affect dynamical indication that this assumption might not hold under all aspects as well as adhesion and wetting characteristic^.^^^ conditions.22 At present it seems to be widely accepted, based on In this study we report how one can use the effect that theoretical con~iderationsl~~ and computer simulations,5-l0 unstable polymer films dewet the substrate as detected that static properties like local density differ from bulk by X-ray reflectometry to learn more about polymer values only up to a few segmental layers away from an density and corresponding glass transition temperature interface. Such conclusions are drawn for both cases, of thin films and about the mobility of polymers within molecules in semiinfinite systems close to an impenetrable such films. interface, or molecules in thin films. Experimentally observed long range forces1'J2 are attributed to pinning 2. Experimental Section of the molecules a t the contact with the wall.I3 Samples and Their Characterization. The investigated Dynamical properties are strongly affected by adsorptive samples consist of polystyrene (PS)films on float glass slides (70 interactions with the substrate and entropic constraints.%l0 x 30 x 4 mm3). Two different molecular weight materials as The mobility of molecules close to a hard wall depends purchased from Polymer Laboratories, U.K., have been used. distinctly on the strength of the interaction with the The polymers were characterized by GPC: PS 28k, M , = 28 000 surface. One reason is that segments touching an attractive gimol, M,IMn = 1.05, REE= 11 nm, TG = 100 "C;PS 660k, M , wall are less mobile (trapped) and thereby slow down the = 660 000 g/mol,MwIMn= 1.1,REE= 54 nm, Tg= 104 "C. M , motion of the whole chain.14J5 Alternatively, strong and M , are weight and number average molecular weight, attraction to the surface might also increase the local respectively. REEis the average end-to-end distance. density and therefore reduce the mobility. In polymer Thin fiims of different thicknesses were prepared by spincoating toluene solutions of various concentrations(1-5 mg/mL) solution this effect of increased density in adsorbed layers at a speed of 2000 rpm onto the substrate. The resulting films is sometimes related to an increased effective glass were checked by X-ray r e f l e c t r ~ m e t r yand ~ ~ interference ,~~ light transition temperature.16 Weak interaction, on the other microsc~py.~~ The polymer density of the thinnest films (after hand, causes a depleted region close to the wall. I t should some annealing) was found to be lower than the bulk value. be mentioned that the influence of an interface is negligible However, the resolution of X-ray reflectrometry with respect to a few segmental diameters away from the interface. polymer density for the present case is rather poor due to the low Confining polymers in a small gap between two walls or scattering contrast between substrate and film. The thickness within thin films on solid substrates can also affect the of the film, on the contrary,can be determined with much higher degree of interpenetration between the m o l e ~ u l e s . ~ J ~ J ~precision (better than 0.1 nm). Interfacialdensity profiles were described by an error-function(standard deviation: a) assuming This can lead to a reduced number of entanglements which Gaussian roughness. The roughness of the air-polymerinterface can cause decreased viscosity and increased diffusivity. was similar to the roughness of the substrate ( g .-5 l o o a ii= c . '
Wavevector k [nm-'1 Figure 6. Same as Figure 5 for an h, = 4.7-nm thick PS660k film. The interference fringes are not damped up to an annealing temperature of T = 85 "C. Dewetting seta in between 85 and 90 "C as the interference pattern of the 90 "C curve is already slightly damped especially at the first minimum at low k values. dewetting, the more appropriate analysis using a profile schematically depicted in Figure I d was performed. Figure 7 shows the hole diameter normalized by its maximum possible value for PS660k samples as a function of film thickness after annealing at two different temperatures. Qualitatively, a roughness interpretation of the damped reflectivity curves would yield a similar trend. However, besides the fact that the used profile is based on the physical origin of the apparent "roughening" of the films, the reflectivity curves can be fitted much better using the dewetting profile. The big advantage of the profile of Figure I d is that it provides direct information on the dynamics of dewetting. Using an error function profile neglects the fact that the number of holes depends significantly on film thickness (2 h-9. This means that
Time [min] Figure 8. (a) Diameter D of holes caused by dewetting versus annealing temperature (annealing time 1h per point) for three different PS660k films. The broken lines indicate the maximum value D can reach. (b)D as a functionof annealingtime (annealing time 90 "C) for three different PS28k films. The broken lines indicate . , D thicker films seem to be stable for a longer period of time simply because there are fewer holes which have to grow much larger to produce the same change in the density profile. Rate of Dewetting. In order to decide how fast the dewetting process takes place the hole diameter D was plotted versus temperature keeping the time constant (Figure 8a) and versus time keeping the annealing temperature constant (Figure 8b). The dewetting velocity u is not constant during the whole dewettingprocess. (Note that the time in Figure 8a is plotted on a logarithmic scale.) u slows down as the height of the rim increases in the course of dewetting. This implies that dewetting a t a constant temperature is faster the thinner the film is. As the average hole diameter reaches its maximum possible value the hole growth slows down drastically and finally stops. Constant temperature experiments demand to vary the time over many orders of magnitude. For the thinnest films dewetting occurs already below TP In order to resolve the dewetting process in time one has to anneal these
Macromolecules, Vol. 27, No. 11, 1994 140 ----I
8 0 1 ,k.A
~ E E,
than in the bulk. The reduction of this transition temperature depends on film thickness, most likely on the ratio of REE/h for h < REE. The results indicate a crossover to bulk behavior happening a t a film thickness which is much more proportional to REEthan to the size of a single segment. Comparison to Bulk. One may quantify the deviation from bulk behavior by comparing the viscosity the polymers of this study show in bulk samples with the value one can estimate from the measured dewetting velocity. According to theoretical considerations38 and recent dewetting experiment^^^ with thick films the dewetting velocity u is related to the viscosity t in the following way.
T. RE, =Y 54n l -
Thickness h, [nm] Figure 9. The dewetting velocity reaches a value of 500 nm/h at a temperature T,. The dependence of T,on the initial thickness (h,) of the films is plotted for (a) PS28k and (b)PS660k. Values expected for bulk-like behavior are indicated by dotted lines. The glass transition temperatures (T,)for bulk samples are marked by broken lines. REE is the end-to-end distance of the molecules. samples below Tg,37However, a t such a temperature thicker films seem to be stable for extremely long times. In fact, the time is certainly longer than several days making constant temperature experiments very difficult. It is not clear if time-temperature superposition applies to our case. We preferred to keep the annealing time constant and interpolate between adjacent temperatures to determine the temperature T, where the dewetting velocity (u = AD/At) has reached a value of 500 nm/h. These temperaturesversus initial film thickness are plotted in Figure 9. We chose this particular value of u for several reasons. D has to be large enough to be detectable even for low hole concentrations. D should be small in order to resolve the onset of dewetting as closely as possible. In the limit u 0 T, is expected to represent the effective glass transition temperture of the films. As it turns out a value of D = 500 nm is small enough to minimize the uncertainty of the onset temperature to a few degrees. Increasing the annealing temperature by a step of 5 deg changes D from zero to several 100 nm within 1 h (one annealing step). Using linear interpolation thus can yield T, better than one annealing step. As can be seen from Figure 9a, T, became independent of h for h larger than about 11 nm for PS28k samples. This thickness compares well to the h, value above which films of PS28k do not change their thickness upon annealing. The PS660k samples do not show such leveling off for T,vs h,. For both molecular weights dewetting was observed below Tg if the film thickness is small enough (< ca. 8 nm).
Effective Glass Transition Temperature of Thin Films. The results of this study clearly show the following tendency. In marked contrast to thicker films the temperature a t which dewetting starta depends significantly on film thickness. For films thinner than about 8 nm dewetting a t a velocity of 500 nm/h occurs even below Tg. Consequently, as dewetting cannot happen when the molecules are in the glassy state, the effective glass transition temperature of polystyrene in thin films is lower
a: is a constant of order 1, y is the surface tension of polystyrene, and 0 is the contact angle polystyrene forms on glass. From eq 11follows that for the chosen velocity (u = 500 nm/h) the viscosity of polystyrene in the film must be approximately lo7 Poise. PS660k and PS28k reach such a value in the bulk a t about 180-190 and 120125 "C,r e ~ p e c t i v e l y . ~Most ~ of the investigated films, however, show this particular value of the viscosity a t much lower temperatures. As an example, PS660k in a 5-nm thick film can reach such a value a t about 90 "C which is about 100 deg below the bulk value. Influence of Molecular Weight. Using two very different molecular weight samples allows to compare the influence of the length of the molecule (or degree of polymerization N ) on viscosity in the bulk and in thin films. For the used samples the viscosity of bulk samples is proportional to IP.4.41At a fixed temperature, the viscosity of PS660k is about 5 X lo4 larger than that of PS28k. Therefore PS660k reaches the same viscosity as PS28k only a t an about 60-70 O C higher temperature. At T, the viscosity is constant. Figure 9 shows that the difference between the T, values of the two molecular weight samples depends on thickness and only for the thickest films approaches the difference in temperature expected for bulk samples. This difference gets very small for the thinnest films. This means that the viscosity of these films becomes less pronounced dependent on N as h decreases. One might explain this behavior by relating it to a decreasing number of entanglements. Density of Thin Polymer Films. The other major result of this study is that the density of thin polymer films decreases with decreasing h. For the thinnest films the reduced density has been detected directly by X-ray reflectometry. However, due to the rather low scattering contrast, the change in density could not be resolved very accurately. In all cases, however, the decrease in density could be calculated from the increase in film thickness. Recent neutron reflectometry measurements which have a much better resolution than the corresponding X-ray measurements, confirmed the relation between thickness increase and density reduction.22 It is worthwhile to note that for PS28k films larger than ca. 11 nm properties like density or dewetting velocity become independent of h. Their thickness does not change upon annealing,and, a t the same time, T,becomes constant a t a value close to what is expected for bulk samples. This indicates the correlation between the reduced density and the increased mobility which, in turn, can be attributed to an effectively lower glass transition temperature. It is well-known that reducing the polymer density by adding a few percent of solvent molecules shifts the glass transition temperature some tens of deg.41 Therefore, explaining
Macromolecules, Vol. 27, No. 11, 1994 why the density of thin polymer films can be lower than in the bulk automatically explains the change in mobility. Improbable Explanations. Two possible explanations of these effects are ruled out. It is known that attractive interactions with the substrate can decrease the mobility of the molecules close to the substrate.14J5 Weak interaction between polymer and substrate might cause a slightly depleted region close to the wall and therefore increase the mobility. However, as the influence of the interface is of short range only, one expects that this effect depends simply on the ratio of surface to volume and therefore should not depend on the length of the molecules. The observed influence of molecular weight thus cannot be explained. One might also assume that the way the films were prepared is responsible for the deviation from bulk behavior. Spin-coating might cause nonequilibrium conformations of the molecules. Recent diffusion experiments indicate that molecules in spin-coated films are less entangled.42 However, after some annealing the molecules will reach equilibrium. Dewetting demands that the molecules move over distances many times their size. Thus, during dewetting the molecules have sufficient time to relax. If their equilibrium properties would be bulk-like, dewetting would have to stop below Tgafter the molecules relaxed. The present experiments, however, show that dewetting continues. For the thinnest films the complete dewetting process occurs below TP Therefore one has to conclude that polymers in thin films have different equilibrium properties, e.g., lower density, than in bulk samples. Segregation of Polymers in Thin Films and Possible Consequences. A comparison of what one knows of polymers in the bulk (we call this the three-dimensional case, assuming h > REE)and what one expects for twodimensional p o l y m e r s ' ~might ~~ help to understand the observed behavior of thin films. Theory1 and computer sir nu la ti on^^^ predict that polymers are highly segregated in two dimensions. An ideal random walk in two dimensions occupies all sites within its perimeter. The square of the end-to-end distance REEis equal to the area of the molecule ( R E E=~ Nu2, u is the length of a segment). Consequently, there is only negligible interpenetration for ideal random walks in two dimensions. We may define the concentration of a particular chain within its envelope volume as the internal concentration 4. For random walks 4 = N-V2 and 4 = 1 in three and two dimensions, respectively. Real polymers cannot cut through themselves, and de Gennes expects that they are slightly swollen in two dimensi0ns.l This is in contrast to the three-dimensional case. As pointed out by F l ~ r ypolymer , ~ ~ melts in three dimensions behave like ideal random walks. This is because longrange interferences between segments of a particular chain cannot be diluted without simultaneously increasing the number of interferences with other molecules. A swelling (or stretching) of the molecules would cost energy that one would not regain from the reduced segmental interferences within a particular chain. One can say that there is effectively no excluded volume for the three-dimensional case. Such a compensation of effects or screening of intramolecular interferences is only possible if the chains are interpenetrating. Confining polymers in films of h < REEleads to a reduction of the interpenetration of molecules. The larger 4 gets the lower is the number of possible paths for other chains through the envelope volume of a particular chain. Interpenetration will cost progressively more entropy the
Dewetting as a Probe of Polymer Mobility in Thin Films 3051 ,higher 4 is, because the penetrating chains have to take conformations which are dictated by the chain they penetrate. If 4 is larger than 1- p c (pCis the percolation threshold for empty sites) there is no continuous path through the envelope volume of a chain.45 Thus there have to be sites which cannot be reached by a chain of connected segments. Only with the help of thermal fluctuations such sites may be reached. This should lead to an even lower interpenetration to polymers. As a consequence not all of the intramolecular interferences can be screened leading to an increase of the excluded volume. It should be noted that in this context the excluded volume is equal (or a t least proportional) to a free or inaccessible volume as it follows from the deficiency of chain interpenetration. The number of inaccessible sites increases with decreasing h, and the overall density of polymers in thin films consequently decreases. This decrease in density is in accordance with the results of this study.
5. Conclusions The purpose of these experiments was to investigate the influence of confinement on static and dynamic behavior of polymers within thin films. It was found that the polymer density of films thinner than their average end-to-end distance is lower than in the bulk in accordance with other studies.22 For thicknesses h < REEthe density decreased with decreasing h. As one might expect, such a reduced density enables molecules to move more easily which can be detected by the onset of dewetting a t temperatures much lower than in bulk samples. Dewetting was detected even below the glass transition temperature in the bulk ( Tg). One can conclude that the effective glass transition temperature of such thin films is lower than Tg.A tentative explanation of the reduced density in thin films is based on packing considerations. Confining polymers in films thinner than REEleads to segregation of the molecules increasing the internal density of each molecule. This increase in internal density, in turn, makes it more difficult for other chains to penetrate into the volume described by the perimeter of the molecules. As a consequence there are inaccessible sites which will stay empty. While such an explanation seems plausible some more elaborate theoretical work is necessary to prove this idea or, alternatively, to explain the experimental results of this study somehow else.
Acknowledgment. I want to thank P. G. de Gennes, E. Raphael, and A. Silberberg for inspiring and helpful discussions. Financial support by BMFT is acknowledged.
References and Notes (1)de Gennes, P. G. Scaling Concepts in Polymer Physics, Cornel1 University Press: Ithaca, NY, 1985. (2) Physics of Polymer Surfaces and Interfaces; Sanchez, I. C., Ed.; Butterworth-Heinemann: Boston, 1992. (3) Liquids at Znterfaces,Proceedingsof the Les Houches Summer School Session X L VZZe Charvolin,J.,Joanny, J.-F.,Zinn-Justin, J., Eds.; Elsevier: Amsterdam, 1989. (4) Ausserr6, D.J . Physique 1989,50, 3021. (5) Kumar, S. K.; Vacatello, M.; Yoon, D. Y. J. Chem. Phys. 1988, 89,5206. (6) ten Brinke, G.; Ausserr6, D.; Hadziioannou, G. J. Chem. Phys. 1988,89,4374. (7) Mansfield,K.;Theodorou,D. N.Macromolecules 1989,22,3143. (8)Yethiraj, A.; Hall, C. K.Macromolecules 1990,23,1865. (9) Bitsanis, I.; Hadziioannou, G. J. Chem. Phys. 1990,92,3827. (10) Smith, G. D.; Yoon, D. Y.; Jaffe, R. L. Macromolecules 1992, 25,7011. (11) Israelachvili, J. N.; Kott, S. J. J . Chem. Phys. 1988,88,7162. Horn, R.G.; Israelachvili, J. N.Macromolecules 1988,21,3143.
Macromolecules, Vol. 27, No. 11, 1994
Hu, H.-W.; Granick, S. Science 1992,258, 1339. de Gennes, P. G. C. R. Acad. Sci. (Paris) 1987,305, 1181. Silberzan, P.; Leger, L. Macromolecules 1992, 25, 1267. Frot, D.; Hervet, H.; Auroy, P.; Leger, L. In Dynamics in Small Confining Systems; Drake, J. M., Klafter, J., Kopelman, R., Eds.; EA-22 Materials Research Society: Pittsburgh, PA, 1990. (16) Kremer, K. J. Physique 1986,47, 1269. (17) Brochard-Wyart, F.; Raphael, E. Macromolecules 1990,23,2276. (18) Brochard, F.; de Gennes, P. G.J .Physique Lett. 1979,40, L-399. (19) Jackson, C. L.;McKenna, G. B. J. Non-Cryst. Solids 1991,131133, 221. (20) Zhang, J.; Liu, G.; Jonas, J. J. Phys. Chem. 1992,96, 3478. (21) Herwig, K. W.; Trouw, F. R. Phys. Reo. Lett. 1992,69, 89. (22) Orts, W. J.; van Zanten, J. H.; Wu, W.-L.; Satija, S. K. Phys. Reo. Lett. 1993, 71, 867. (23) Foster, M.; Stamm, M.; Reiter, G.; Huttenbach, S. Vacuum 1990,41, 1441. (24) Russell, T. P. Mat. Rep. 1990,5, 171. ( 2 5 ) Biegen, J. F.; Smythe, R. A. Proceedings of the SPIE O/E L A S E 8 4 Los Angeles, CA, 1988. (26) Robbins, M. O.;Andelman, D.; Joanny, J. F. Phys. Reo. A 1991, 43, 4344. (27) Tidswell, I. M.; Rabedeau, T. A.; Pershan, P. S.; Kosowsky, S. D. Phys. Reo. Lett. 1991,66, 2108. (28) Reiter, G. Phys. Reo. Lett. 1992, 68, 75. (29) Reiter, G. Langmuir 1993, 9, 1344. (30) The prefactor fl comes from a fit to the data of NH vs h in Figure 10 of ref 29. The area/hole = l/@h4, the maximum diameter of an average hole is proportional to (area/hole)*/Z. (31) Detectability by X-ray reflectrometry depends on film thickness as the necessary change in electron density is proportional to the number of holes 2 oh4. (12) (13) (14) (15)
(32) From experiments with much thicker films (20-200 nm for PS28k,28.as35-200 nm for PS66Oka) of the same molecules it is known that the thickness of such films does not change by more than 0 . 1 4 2 nm upon annealing. In many cases h slightly decreased (-0.1 nm) which might be attributed to evaporation of residual solvent. (33) Reiter, G.; Steiner, U. J. Physique ZZ 1991, I, 659. (34) Approximately 3-4 nm seems to be the minimum thickness of a polystyrene film which can be prepared by spin-coating. This is in accordance with the results of an earlier AFM study.% (35) Stange, T. G.; Mathew, R.; Evans, D. F.; Hendrickson, W. A. Langmuir 1992,8, 920. (36) Zhao, W.; Rafailovich, M. H.; Sokolov,J.; Fetters, L. J.; Plano, R.; Sanyal, M. K.; Sinha, S. K.; Sauer, B. B. Phys. Rev. Lett. 1993, 70, 1453. (37) Annealing times shorter than -15 min are not used because the glass substrates cannot reach the oven temperature very fast due to their bad thermal conductivity. (38) Brochard-Wyart, F.; Daillant, J. Can. J. Phys. 1990,68, 1084. (39) Redon, C.; Brochard-Wyart, F.; Rondelez, F. Phys. Reo. Lett. 1991, 66, 715. (40) Plazek, D. J.; O’Rourke, V. M. J. Polym. Sci., Part A-2 1971, 9, 209. (41) Ferry, J. D. Viscoelastic Properties of Polymers; Wiley: New York, 1980. (42) Sauer, B. B.; Walsh, D. J. Preprint. (43) Carmesin, I.; Kremer, K. J. Physique 1990, 51, 915. (44) Flory, P. J. J. Chem. Phys. 1949,17,303. (45) Stauffer, D.; Aharoni, A. Introduction to Percolation Theory; Taylor & Francis: London, 1992.